# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_NaBiBaO
_database_code_depnum_ccdc_archive 'CCDC 2119540'
loop_
_audit_author_name
_audit_author_address
'Nobuhiro Kumada'
;University of Yamanashi
Japan
;
_audit_update_record             
;
2021-10-30 deposited with the CCDC.	2022-01-20 downloaded from the CCDC.
;
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Ba4 Bi3 Na O12'
_chemical_formula_iupac          ?
_chemical_formula_weight         1391.29

_chemical_melting_point          ?

_space_group_crystal_system      triclinic
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   8.5415(2)
_cell_length_b                   8.5421(2)
_cell_length_c                   8.5441(2)
_cell_angle_alpha                89.9960(10)
_cell_angle_beta                 89.9950(10)
_cell_angle_gamma                90.0160(10)
_cell_volume                     623.40(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9958
_cell_measurement_theta_min      3.3725
_cell_measurement_theta_max      27.478
_cell_measurement_temperature    298.(2)

_exptl_crystal_description       ochahedron
_exptl_crystal_colour            black
_exptl_crystal_size_max          0.039
_exptl_crystal_size_mid          0.038
_exptl_crystal_size_min          0.036
_exptl_crystal_density_diffrn    7.412
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1160

_exptl_absorpt_coefficient_mu    54.702
_exptl_absorpt_correction_type   Multi-Scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 - Bruker AXS area detector scaling and absorption correction
;
_exptl_absorpt_correction_T_min  0.0587
_exptl_absorpt_correction_T_max  0.0887

_exptl_special_details           
;
;

_diffrn_ambient_temperature      298.(2)

_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'micro focus sealed tube'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'

_diffrn_detector_area_resol_mean 7.3910

_diffrn_reflns_number            21936
_diffrn_reflns_av_R_equivalents  0.0249
_diffrn_reflns_av_unetI/netI     0.0199
_diffrn_reflns_theta_min         2.38
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_full        27.48
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       11

_refine_special_details          
;

Refined as a 2-component inversion twin.
;

_reflns_number_total             2866
_reflns_number_gt                2446
_reflns_threshold_expression     'I > 2σ(I)'

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_R_factor_all          0.0234
_refine_ls_R_factor_gt           0.0202
_refine_ls_wR_factor_gt          0.0450
_refine_ls_wR_factor_ref         0.0476
_refine_ls_goodness_of_fit_ref   1.167
_refine_ls_restrained_S_all      1.166
_refine_ls_number_reflns         2866
_refine_ls_number_parameters     141
_refine_ls_number_restraints     1
_refine_ls_number_constraints    ?
_refine_ls_hydrogen_treatment    undef
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0149P)²+2.3539P] where P=(Fo²+2Fc²)/3'

_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_diff_density_max         1.575
_refine_diff_density_min         -1.230
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_extinction_coef       0.00138(7)

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_computing_data_collection       'Bruker Instrument Service vV6.2.9'
_computing_cell_refinement       'APEX3 v2018.1-0 (Bruker AXS)'
_computing_data_reduction        'SAINT V8.38A (Bruker AXS Inc., 2017)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    'VESTA v2.1.6 (Momma & Izumi, 2011)'
_computing_publication_material  ?

loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_refinement_flags_posn
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Na Na1 0 0.5 0.5 0.0121(8) Uani d . P S 0.896(2) . .
Bi Bi1 0 0.5 0.5 0.0121(8) Uani d . P S 0.104(2) . .
Na Na2 0.5 0 0 0.0150(9) Uani d . P S 0.897(2) . .
Bi Bi2 0.5 0 0 0.0150(9) Uani d . P S 0.103(2) . .
Na Na3 0 0 0.5 0.00825(14) Uani d . P S 0.0398(15) . .
Bi Bi3 0 0 0.5 0.00825(14) Uani d . P S 0.9602(15) . .
Na Na4 0.5 0.5 0 0.00839(14) Uani d . P S 0.0432(15) . .
Bi Bi4 0.5 0.5 0 0.00839(14) Uani d . P S 0.9568(15) . .
Na Na7 0.5 0.5 0.5 0.0101(4) Uani d . P S 0.0631(18) . .
Bi Bi7 0.5 0.5 0.5 0.0101(4) Uani d . P S 0.9369(18) . .
Na Na8 0 0 0 0.0106(4) Uani d . P S 0.0604(18) . .
Bi Bi8 0 0 0 0.0106(4) Uani d . P S 0.9396(18) . .
Bi Bi5 0.5 0 0.5 0.0100(4) Uani d . P S 1.0 . .
Bi Bi6 0 0.5 0 0.0102(4) Uani d . P S 1.0 . .
Ba Ba1 0.25113(7) 0.75094(5) 0.25029(6) 0.0271(4) Uani d . . . 1.0 . .
Ba Ba2 0.24917(7) 0.25072(5) 0.24890(6) 0.0270(4) Uani d . . . 1.0 . .
Ba Ba3 0.24968(6) 0.74945(4) 0.75019(5) 0.0118(3) Uani d . . . 1.0 . .
Ba Ba4 0.25001(6) 0.24939(4) 0.74878(5) 0.0115(3) Uani d . . . 1.0 . .
O O1 0.5128(7) 0.9789(6) 0.2684(7) 0.0218(12) Uiso d . . . 1.0 . .
O O2 -0.0108(7) 0.4802(6) 0.2316(7) 0.0203(12) Uiso d . . . 1.0 . .
O O3 -0.0035(7) 0.2324(4) 0.5279(5) 0.0165(8) Uiso d . . . 1.0 . .
O O4 0.5037(7) 0.7328(4) 0.9733(5) 0.0160(8) Uiso d . . . 1.0 . .
O O5 0.2661(10) 0.4963(9) 0.5111(9) 0.0372(18) Uiso d . . . 1.0 . .
O O6 0.2322(8) -0.0027(7) -0.0173(7) 0.0238(14) Uiso d . . . 1.0 . .
O O7 0.2499(8) 1.0035(7) 0.4810(7) 0.0282(15) Uiso d . . . 1.0 . .
O O8 0.2474(9) 0.5035(8) 0.0106(9) 0.042(2) Uiso d . . . 1.0 . .
O O9 1.0107(7) 0.0248(7) 0.2495(7) 0.0242(12) Uiso d . . . 1.0 . .
O O10 0.4867(7) 0.5235(6) 0.2490(7) 0.0225(12) Uiso d . . . 1.0 . .
O O11 0.5029(8) 0.2495(7) 0.4683(5) 0.0191(8) Uiso d . . . 1.0 . .
O O12 -0.0037(8) 0.7492(7) 0.0291(5) 0.0166(8) Uiso d . . . 1.0 . .


_geom_special_details            
;

All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix.  The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry.  An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Bi1 O5 2_566 2.275(8) ?
Bi1 O5 . 2.275(8) ?
Bi1 O3 . 2.298(4) ?
Bi1 O3 2_566 2.298(4) ?
Bi1 O2 . 2.301(6) ?
Bi1 O2 2_566 2.301(6) ?
Bi1 Ba3 2_566 3.6955(3) ?
Bi1 Ba3 . 3.6955(3) ?
Bi1 Ba4 . 3.6964(4) ?
Bi1 Ba4 2_566 3.6965(4) ?
Bi1 Ba2 2_566 3.6972(7) ?
Bi1 Ba2 . 3.6972(7) ?
Bi2 O6 2_655 2.293(7) ?
Bi2 O6 . 2.293(7) ?
Bi2 O4 2_666 2.294(4) ?
Bi2 O4 1_544 2.294(4) ?
Bi2 O1 2_665 2.303(6) ?
Bi2 O1 1_545 2.303(6) ?
Bi2 Ba1 1_545 3.6898(7) ?
Bi2 Ba1 2_665 3.6898(7) ?
Bi2 Ba2 . 3.7016(7) ?
Bi2 Ba2 2_655 3.7016(7) ?
Bi2 Ba3 2_666 3.7023(3) ?
Bi2 Ba3 1_544 3.7023(3) ?
Bi3 O3 2_556 2.000(4) ?
Bi3 O3 . 2.000(4) ?
Bi3 O7 2_566 2.141(7) ?
Bi3 O7 1_545 2.141(7) ?
Bi3 O9 2_656 2.153(6) ?
Bi3 O9 1_455 2.153(6) ?
Bi3 Ba4 2_556 3.6899(3) ?
Bi3 Ba4 . 3.6899(3) ?
Bi3 Ba1 2_566 3.6988(6) ?
Bi3 Ba1 1_545 3.6988(6) ?
Bi3 Ba3 1_545 3.7014(3) ?
Bi3 Ba3 2_566 3.7014(3) ?
Bi4 O4 2_666 2.002(4) ?
Bi4 O4 1_554 2.002(4) ?
Bi4 O10 . 2.140(6) ?
Bi4 O10 2_665 2.140(6) ?
Bi4 O8 . 2.160(8) ?
Bi4 O8 2_665 2.160(8) ?
Bi4 Ba2 . 3.6937(6) ?
Bi4 Ba2 2_665 3.6937(6) ?
Bi4 Ba3 2_666 3.6974(3) ?
Bi4 Ba3 1_554 3.6974(3) ?
Bi4 Ba1 . 3.6999(6) ?
Bi4 Ba1 2_665 3.6999(6) ?
Bi7 O5 . 2.001(8) ?
Bi7 O5 2_666 2.001(8) ?
Bi7 O11 2_666 2.157(6) ?
Bi7 O11 . 2.157(6) ?
Bi7 O10 2_666 2.157(6) ?
Bi7 O10 . 2.157(6) ?
Bi7 Ba4 2_666 3.6954(5) ?
Bi7 Ba4 . 3.6954(5) ?
Bi7 Ba1 2_666 3.6971(4) ?
Bi7 Ba1 . 3.6971(4) ?
Bi7 Ba3 . 3.6992(5) ?
Bi7 Ba3 2_666 3.6992(5) ?
Bi8 O6 . 1.989(7) ?
Bi8 O6 2 1.989(7) ?
Bi8 O9 2_655 2.144(6) ?
Bi8 O9 1_455 2.144(6) ?
Bi8 O12 2_565 2.157(6) ?
Bi8 O12 1_545 2.157(6) ?
Bi8 Ba2 . 3.6929(4) ?
Bi8 Ba2 2 3.6929(4) ?
Bi8 Ba3 1_544 3.6996(5) ?
Bi8 Ba3 2_566 3.6996(5) ?
Bi8 Ba4 1_554 3.7016(5) ?
Bi8 Ba4 2_556 3.7016(5) ?
Bi5 O1 2_666 1.990(6) ?
Bi5 O1 1_545 1.990(6) ?
Bi5 O7 2_666 2.143(7) ?
Bi5 O7 1_545 2.143(7) ?
Bi5 O11 . 2.149(6) ?
Bi5 O11 2_656 2.149(6) ?
Bi5 Ba1 2_666 3.6872(4) ?
Bi5 Ba1 1_545 3.6872(4) ?
Bi5 Ba4 2_656 3.6902(5) ?
Bi5 Ba4 . 3.6903(5) ?
Bi5 Ba3 1_545 3.7037(5) ?
Bi5 Ba3 2_666 3.7037(5) ?
Bi6 O2 2_565 1.988(6) ?
Bi6 O2 . 1.988(6) ?
Bi6 O8 2_565 2.115(8) ?
Bi6 O8 . 2.115(8) ?
Bi6 O12 . 2.143(6) ?
Bi6 O12 2_565 2.143(6) ?
Bi6 Ba2 2_565 3.6863(4) ?
Bi6 Ba2 . 3.6864(4) ?
Bi6 Ba3 1_554 3.6933(5) ?
Bi6 Ba3 2_566 3.6933(5) ?
Bi6 Ba4 1_554 3.7085(5) ?
Bi6 Ba4 2_566 3.7085(5) ?
Ba1 O10 . 2.797(6) ?
Ba1 O3 2_566 2.843(6) ?
Ba1 O12 . 2.882(5) ?
Ba1 O7 . 2.923(6) ?
Ba1 O8 . 2.943(8) ?
Ba1 O1 . 2.968(5) ?
Ba1 O6 1_565 3.111(6) ?
Ba1 O9 1_465 3.113(6) ?
Ba1 O5 . 3.117(8) ?
Ba1 O11 2_666 3.193(5) ?
Ba1 O4 1_554 3.206(5) ?
Ba1 O2 . 3.221(6) ?
Ba2 O9 1_455 2.806(6) ?
Ba2 O4 2_666 2.842(6) ?
Ba2 O11 . 2.866(6) ?
Ba2 O7 1_545 2.897(6) ?
Ba2 O2 . 2.966(5) ?
Ba2 O8 . 2.968(7) ?
Ba2 O5 . 3.072(7) ?
Ba2 O10 . 3.090(5) ?
Ba2 O6 . 3.143(6) ?
Ba2 O12 2_565 3.169(5) ?
Ba2 O3 . 3.219(6) ?
Ba2 O1 1_545 3.239(6) ?
Ba3 O11 2_666 2.819(6) ?
Ba3 O2 2_566 2.834(6) ?
Ba3 O4 . 2.892(5) ?
Ba3 O6 1_566 2.907(6) ?
Ba3 O9 2_666 2.944(6) ?
Ba3 O5 . 2.978(7) ?
Ba3 O8 1_556 3.060(7) ?
Ba3 O1 2_676 3.085(5) ?
Ba3 O7 . 3.162(6) ?
Ba3 O3 2_566 3.176(5) ?
Ba3 O12 1_556 3.219(5) ?
Ba3 O10 2_666 3.242(6) ?
Ba4 O1 2_666 2.816(6) ?
Ba4 O12 2_566 2.834(6) ?
Ba4 O3 . 2.877(5) ?
Ba4 O5 . 2.931(8) ?
Ba4 O6 1_556 2.942(6) ?
Ba4 O10 2_666 2.969(5) ?
Ba4 O2 2_566 3.088(5) ?
Ba4 O7 1_545 3.106(6) ?
Ba4 O8 1_556 3.117(8) ?
Ba4 O4 2_667 3.176(5) ?
Ba4 O11 . 3.227(6) ?
Ba4 O9 2_656 3.231(6) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O5 Bi1 O5 2_566 . 180.0 ?
O5 Bi1 O3 2_566 . 90.31(19) ?
O5 Bi1 O3 . . 89.69(19) ?
O5 Bi1 O3 2_566 2_566 89.69(19) ?
O5 Bi1 O3 . 2_566 90.31(19) ?
O3 Bi1 O3 . 2_566 180.0 ?
O5 Bi1 O2 2_566 . 85.4(3) ?
O5 Bi1 O2 . . 94.6(3) ?
O3 Bi1 O2 . . 91.70(16) ?
O3 Bi1 O2 2_566 . 88.30(16) ?
O5 Bi1 O2 2_566 2_566 94.6(3) ?
O5 Bi1 O2 . 2_566 85.4(3) ?
O3 Bi1 O2 . 2_566 88.30(16) ?
O3 Bi1 O2 2_566 2_566 91.70(16) ?
O2 Bi1 O2 . 2_566 180.0 ?
O5 Bi1 Ba3 2_566 2_566 53.67(19) ?
O5 Bi1 Ba3 . 2_566 126.33(19) ?
O3 Bi1 Ba3 . 2_566 58.60(13) ?
O3 Bi1 Ba3 2_566 2_566 121.40(13) ?
O2 Bi1 Ba3 . 2_566 50.06(14) ?
O2 Bi1 Ba3 2_566 2_566 129.94(14) ?
O5 Bi1 Ba3 2_566 . 126.33(19) ?
O5 Bi1 Ba3 . . 53.67(19) ?
O3 Bi1 Ba3 . . 121.40(13) ?
O3 Bi1 Ba3 2_566 . 58.60(13) ?
O2 Bi1 Ba3 . . 129.94(14) ?
O2 Bi1 Ba3 2_566 . 50.06(14) ?
Ba3 Bi1 Ba3 2_566 . 180.0 ?
O5 Bi1 Ba4 2_566 . 127.55(19) ?
O5 Bi1 Ba4 . . 52.45(19) ?
O3 Bi1 Ba4 . . 51.10(13) ?
O3 Bi1 Ba4 2_566 . 128.91(13) ?
O2 Bi1 Ba4 . . 123.62(13) ?
O2 Bi1 Ba4 2_566 . 56.38(13) ?
Ba3 Bi1 Ba4 2_566 . 109.398(8) ?
Ba3 Bi1 Ba4 . . 70.601(8) ?
O5 Bi1 Ba4 2_566 2_566 52.45(19) ?
O5 Bi1 Ba4 . 2_566 127.55(19) ?
O3 Bi1 Ba4 . 2_566 128.91(13) ?
O3 Bi1 Ba4 2_566 2_566 51.09(13) ?
O2 Bi1 Ba4 . 2_566 56.38(13) ?
O2 Bi1 Ba4 2_566 2_566 123.62(13) ?
Ba3 Bi1 Ba4 2_566 2_566 70.602(8) ?
Ba3 Bi1 Ba4 . 2_566 109.398(8) ?
Ba4 Bi1 Ba4 . 2_566 180.0 ?
O5 Bi1 Ba2 2_566 2_566 56.01(19) ?
O5 Bi1 Ba2 . 2_566 123.99(19) ?
O3 Bi1 Ba2 . 2_566 120.35(14) ?
O3 Bi1 Ba2 2_566 2_566 59.65(14) ?
O2 Bi1 Ba2 . 2_566 126.68(13) ?
O2 Bi1 Ba2 2_566 2_566 53.32(13) ?
Ba3 Bi1 Ba2 2_566 2_566 109.610(8) ?
Ba3 Bi1 Ba2 . 2_566 70.391(8) ?
Ba4 Bi1 Ba2 . 2_566 109.428(11) ?
Ba4 Bi1 Ba2 2_566 2_566 70.572(11) ?
O5 Bi1 Ba2 2_566 . 123.99(19) ?
O5 Bi1 Ba2 . . 56.01(19) ?
O3 Bi1 Ba2 . . 59.65(14) ?
O3 Bi1 Ba2 2_566 . 120.35(14) ?
O2 Bi1 Ba2 . . 53.32(13) ?
O2 Bi1 Ba2 2_566 . 126.68(13) ?
Ba3 Bi1 Ba2 2_566 . 70.391(8) ?
Ba3 Bi1 Ba2 . . 109.609(8) ?
Ba4 Bi1 Ba2 . . 70.572(11) ?
Ba4 Bi1 Ba2 2_566 . 109.428(11) ?
Ba2 Bi1 Ba2 2_566 . 180.0 ?
O6 Bi2 O6 2_655 . 180.0 ?
O6 Bi2 O4 2_655 2_666 89.87(17) ?
O6 Bi2 O4 . 2_666 90.13(17) ?
O6 Bi2 O4 2_655 1_544 90.13(17) ?
O6 Bi2 O4 . 1_544 89.87(17) ?
O4 Bi2 O4 2_666 1_544 180.0 ?
O6 Bi2 O1 2_655 2_665 96.4(2) ?
O6 Bi2 O1 . 2_665 83.6(2) ?
O4 Bi2 O1 2_666 2_665 91.19(16) ?
O4 Bi2 O1 1_544 2_665 88.81(16) ?
O6 Bi2 O1 2_655 1_545 83.6(2) ?
O6 Bi2 O1 . 1_545 96.4(2) ?
O4 Bi2 O1 2_666 1_545 88.81(16) ?
O4 Bi2 O1 1_544 1_545 91.19(16) ?
O1 Bi2 O1 2_665 1_545 180.0(4) ?
O6 Bi2 Ba1 2_655 1_545 122.90(15) ?
O6 Bi2 Ba1 . 1_545 57.10(15) ?
O4 Bi2 Ba1 2_666 1_545 120.51(13) ?
O4 Bi2 Ba1 1_544 1_545 59.49(13) ?
O1 Bi2 Ba1 2_665 1_545 126.49(13) ?
O1 Bi2 Ba1 1_545 1_545 53.51(13) ?
O6 Bi2 Ba1 2_655 2_665 57.10(15) ?
O6 Bi2 Ba1 . 2_665 122.90(15) ?
O4 Bi2 Ba1 2_666 2_665 59.49(13) ?
O4 Bi2 Ba1 1_544 2_665 120.51(13) ?
O1 Bi2 Ba1 2_665 2_665 53.51(13) ?
O1 Bi2 Ba1 1_545 2_665 126.49(13) ?
Ba1 Bi2 Ba1 1_545 2_665 180.0 ?
O6 Bi2 Ba2 2_655 . 122.33(15) ?
O6 Bi2 Ba2 . . 57.67(15) ?
O4 Bi2 Ba2 2_666 . 50.13(14) ?
O4 Bi2 Ba2 1_544 . 129.87(14) ?
O1 Bi2 Ba2 2_665 . 119.95(14) ?
O1 Bi2 Ba2 1_545 . 60.05(14) ?
Ba1 Bi2 Ba2 1_545 . 70.562(10) ?
Ba1 Bi2 Ba2 2_665 . 109.438(10) ?
O6 Bi2 Ba2 2_655 2_655 57.67(15) ?
O6 Bi2 Ba2 . 2_655 122.33(15) ?
O4 Bi2 Ba2 2_666 2_655 129.87(14) ?
O4 Bi2 Ba2 1_544 2_655 50.13(14) ?
O1 Bi2 Ba2 2_665 2_655 60.05(14) ?
O1 Bi2 Ba2 1_545 2_655 119.95(14) ?
Ba1 Bi2 Ba2 1_545 2_655 109.438(10) ?
Ba1 Bi2 Ba2 2_665 2_655 70.562(10) ?
Ba2 Bi2 Ba2 . 2_655 180.0 ?
O6 Bi2 Ba3 2_655 2_666 51.74(15) ?
O6 Bi2 Ba3 . 2_666 128.26(15) ?
O4 Bi2 Ba3 2_666 2_666 51.36(13) ?
O4 Bi2 Ba3 1_544 2_666 128.64(13) ?
O1 Bi2 Ba3 2_665 2_666 123.82(13) ?
O1 Bi2 Ba3 1_545 2_666 56.18(13) ?
Ba1 Bi2 Ba3 1_545 2_666 109.372(10) ?
Ba1 Bi2 Ba3 2_665 2_666 70.628(10) ?
Ba2 Bi2 Ba3 . 2_666 70.643(8) ?
Ba2 Bi2 Ba3 2_655 2_666 109.357(8) ?
O6 Bi2 Ba3 2_655 1_544 128.26(15) ?
O6 Bi2 Ba3 . 1_544 51.74(15) ?
O4 Bi2 Ba3 2_666 1_544 128.64(13) ?
O4 Bi2 Ba3 1_544 1_544 51.36(13) ?
O1 Bi2 Ba3 2_665 1_544 56.18(13) ?
O1 Bi2 Ba3 1_545 1_544 123.82(13) ?
Ba1 Bi2 Ba3 1_545 1_544 70.628(10) ?
Ba1 Bi2 Ba3 2_665 1_544 109.372(10) ?
Ba2 Bi2 Ba3 . 1_544 109.357(8) ?
Ba2 Bi2 Ba3 2_655 1_544 70.643(8) ?
Ba3 Bi2 Ba3 2_666 1_544 180.000(13) ?
O3 Bi3 O3 2_556 . 180.0 ?
O3 Bi3 O7 2_556 2_566 90.6(2) ?
O3 Bi3 O7 . 2_566 89.4(2) ?
O3 Bi3 O7 2_556 1_545 89.4(2) ?
O3 Bi3 O7 . 1_545 90.6(2) ?
O7 Bi3 O7 2_566 1_545 180.00(3) ?
O3 Bi3 O9 2_556 2_656 91.2(2) ?
O3 Bi3 O9 . 2_656 88.8(2) ?
O7 Bi3 O9 2_566 2_656 83.2(3) ?
O7 Bi3 O9 1_545 2_656 96.8(3) ?
O3 Bi3 O9 2_556 1_455 88.8(2) ?
O3 Bi3 O9 . 1_455 91.2(2) ?
O7 Bi3 O9 2_566 1_455 96.8(3) ?
O7 Bi3 O9 1_545 1_455 83.2(3) ?
O9 Bi3 O9 2_656 1_455 180.0 ?
O3 Bi3 Ba4 2_556 2_556 50.74(15) ?
O3 Bi3 Ba4 . 2_556 129.26(15) ?
O7 Bi3 Ba4 2_566 2_556 57.22(16) ?
O7 Bi3 Ba4 1_545 2_556 122.78(16) ?
O9 Bi3 Ba4 2_656 2_556 119.44(16) ?
O9 Bi3 Ba4 1_455 2_556 60.56(16) ?
O3 Bi3 Ba4 2_556 . 129.26(15) ?
O3 Bi3 Ba4 . . 50.74(15) ?
O7 Bi3 Ba4 2_566 . 122.78(16) ?
O7 Bi3 Ba4 1_545 . 57.22(16) ?
O9 Bi3 Ba4 2_656 . 60.56(16) ?
O9 Bi3 Ba4 1_455 . 119.44(16) ?
Ba4 Bi3 Ba4 2_556 . 180.0 ?
O3 Bi3 Ba1 2_556 2_566 130.44(17) ?
O3 Bi3 Ba1 . 2_566 49.56(17) ?
O7 Bi3 Ba1 2_566 2_566 52.13(16) ?
O7 Bi3 Ba1 1_545 2_566 127.87(16) ?
O9 Bi3 Ba1 2_656 2_566 57.22(15) ?
O9 Bi3 Ba1 1_455 2_566 122.78(15) ?
Ba4 Bi3 Ba1 2_556 2_566 109.193(8) ?
Ba4 Bi3 Ba1 . 2_566 70.806(8) ?
O3 Bi3 Ba1 2_556 1_545 49.56(17) ?
O3 Bi3 Ba1 . 1_545 130.44(17) ?
O7 Bi3 Ba1 2_566 1_545 127.87(16) ?
O7 Bi3 Ba1 1_545 1_545 52.13(16) ?
O9 Bi3 Ba1 2_656 1_545 122.78(15) ?
O9 Bi3 Ba1 1_455 1_545 57.22(15) ?
Ba4 Bi3 Ba1 2_556 1_545 70.807(8) ?
Ba4 Bi3 Ba1 . 1_545 109.194(8) ?
Ba1 Bi3 Ba1 2_566 1_545 180.0 ?
O3 Bi3 Ba3 2_556 1_545 59.06(14) ?
O3 Bi3 Ba3 . 1_545 120.94(14) ?
O7 Bi3 Ba3 2_566 1_545 121.52(17) ?
O7 Bi3 Ba3 1_545 1_545 58.48(17) ?
O9 Bi3 Ba3 2_656 1_545 52.65(15) ?
O9 Bi3 Ba3 1_455 1_545 127.35(15) ?
Ba4 Bi3 Ba3 2_556 1_545 109.411(8) ?
Ba4 Bi3 Ba3 . 1_545 70.589(8) ?
Ba1 Bi3 Ba3 2_566 1_545 109.498(10) ?
Ba1 Bi3 Ba3 1_545 1_545 70.502(10) ?
O3 Bi3 Ba3 2_556 2_566 120.94(14) ?
O3 Bi3 Ba3 . 2_566 59.06(14) ?
O7 Bi3 Ba3 2_566 2_566 58.48(17) ?
O7 Bi3 Ba3 1_545 2_566 121.52(17) ?
O9 Bi3 Ba3 2_656 2_566 127.35(15) ?
O9 Bi3 Ba3 1_455 2_566 52.65(15) ?
Ba4 Bi3 Ba3 2_556 2_566 70.589(8) ?
Ba4 Bi3 Ba3 . 2_566 109.411(8) ?
Ba1 Bi3 Ba3 2_566 2_566 70.502(10) ?
Ba1 Bi3 Ba3 1_545 2_566 109.498(10) ?
Ba3 Bi3 Ba3 1_545 2_566 180.0 ?
O4 Bi4 O4 2_666 1_554 180.00(2) ?
O4 Bi4 O10 2_666 . 88.81(19) ?
O4 Bi4 O10 1_554 . 91.19(19) ?
O4 Bi4 O10 2_666 2_665 91.19(19) ?
O4 Bi4 O10 1_554 2_665 88.81(19) ?
O10 Bi4 O10 . 2_665 180.00(3) ?
O4 Bi4 O8 2_666 . 89.6(2) ?
O4 Bi4 O8 1_554 . 90.4(2) ?
O10 Bi4 O8 . . 84.5(3) ?
O10 Bi4 O8 2_665 . 95.5(3) ?
O4 Bi4 O8 2_666 2_665 90.4(2) ?
O4 Bi4 O8 1_554 2_665 89.6(2) ?
O10 Bi4 O8 . 2_665 95.5(3) ?
O10 Bi4 O8 2_665 2_665 84.5(3) ?
O8 Bi4 O8 . 2_665 180.0 ?
O4 Bi4 Ba2 2_666 . 49.65(16) ?
O4 Bi4 Ba2 1_554 . 130.35(16) ?
O10 Bi4 Ba2 . . 56.71(14) ?
O10 Bi4 Ba2 2_665 . 123.29(14) ?
O8 Bi4 Ba2 . . 53.5(2) ?
O8 Bi4 Ba2 2_665 . 126.5(2) ?
O4 Bi4 Ba2 2_666 2_665 130.35(16) ?
O4 Bi4 Ba2 1_554 2_665 49.65(16) ?
O10 Bi4 Ba2 . 2_665 123.29(14) ?
O10 Bi4 Ba2 2_665 2_665 56.71(14) ?
O8 Bi4 Ba2 . 2_665 126.5(2) ?
O8 Bi4 Ba2 2_665 2_665 53.5(2) ?
Ba2 Bi4 Ba2 . 2_665 180.0 ?
O4 Bi4 Ba3 2_666 2_666 51.01(15) ?
O4 Bi4 Ba3 1_554 2_666 128.99(15) ?
O10 Bi4 Ba3 . 2_666 60.72(16) ?
O10 Bi4 Ba3 2_665 2_666 119.28(16) ?
O8 Bi4 Ba3 . 2_666 124.2(2) ?
O8 Bi4 Ba3 2_665 2_666 55.8(2) ?
Ba2 Bi4 Ba3 . 2_666 70.784(9) ?
Ba2 Bi4 Ba3 2_665 2_666 109.216(9) ?
O4 Bi4 Ba3 2_666 1_554 128.99(15) ?
O4 Bi4 Ba3 1_554 1_554 51.01(15) ?
O10 Bi4 Ba3 . 1_554 119.28(16) ?
O10 Bi4 Ba3 2_665 1_554 60.72(16) ?
O8 Bi4 Ba3 . 1_554 55.8(2) ?
O8 Bi4 Ba3 2_665 1_554 124.2(2) ?
Ba2 Bi4 Ba3 . 1_554 109.216(9) ?
Ba2 Bi4 Ba3 2_665 1_554 70.784(9) ?
Ba3 Bi4 Ba3 2_666 1_554 180.0 ?
O4 Bi4 Ba1 2_666 . 120.04(15) ?
O4 Bi4 Ba1 1_554 . 59.96(15) ?
O10 Bi4 Ba1 . . 48.73(16) ?
O10 Bi4 Ba1 2_665 . 131.27(16) ?
O8 Bi4 Ba1 . . 52.7(2) ?
O8 Bi4 Ba1 2_665 . 127.3(2) ?
Ba2 Bi4 Ba1 . . 70.611(12) ?
Ba2 Bi4 Ba1 2_665 . 109.389(12) ?
Ba3 Bi4 Ba1 2_666 . 109.430(10) ?
Ba3 Bi4 Ba1 1_554 . 70.570(11) ?
O4 Bi4 Ba1 2_666 2_665 59.96(15) ?
O4 Bi4 Ba1 1_554 2_665 120.04(15) ?
O10 Bi4 Ba1 . 2_665 131.27(16) ?
O10 Bi4 Ba1 2_665 2_665 48.73(16) ?
O8 Bi4 Ba1 . 2_665 127.3(2) ?
O8 Bi4 Ba1 2_665 2_665 52.7(2) ?
Ba2 Bi4 Ba1 . 2_665 109.389(12) ?
Ba2 Bi4 Ba1 2_665 2_665 70.611(12) ?
Ba3 Bi4 Ba1 2_666 2_665 70.570(10) ?
Ba3 Bi4 Ba1 1_554 2_665 109.430(10) ?
Ba1 Bi4 Ba1 . 2_665 180.0 ?
O5 Bi7 O5 . 2_666 180.0 ?
O5 Bi7 O11 . 2_666 89.9(2) ?
O5 Bi7 O11 2_666 2_666 90.1(2) ?
O5 Bi7 O11 . . 90.1(2) ?
O5 Bi7 O11 2_666 . 89.9(2) ?
O11 Bi7 O11 2_666 . 180.0 ?
O5 Bi7 O10 . 2_666 90.2(2) ?
O5 Bi7 O10 2_666 2_666 89.8(2) ?
O11 Bi7 O10 2_666 2_666 88.17(19) ?
O11 Bi7 O10 . 2_666 91.83(19) ?
O5 Bi7 O10 . . 89.8(2) ?
O5 Bi7 O10 2_666 . 90.2(2) ?
O11 Bi7 O10 2_666 . 91.83(19) ?
O11 Bi7 O10 . . 88.17(19) ?
O10 Bi7 O10 2_666 . 180.0 ?
O5 Bi7 Ba4 . 2_666 127.8(2) ?
O5 Bi7 Ba4 2_666 2_666 52.2(2) ?
O11 Bi7 Ba4 2_666 2_666 60.30(15) ?
O11 Bi7 Ba4 . 2_666 119.70(15) ?
O10 Bi7 Ba4 2_666 2_666 126.54(15) ?
O10 Bi7 Ba4 . 2_666 53.46(15) ?
O5 Bi7 Ba4 . . 52.2(2) ?
O5 Bi7 Ba4 2_666 . 127.8(2) ?
O11 Bi7 Ba4 2_666 . 119.70(15) ?
O11 Bi7 Ba4 . . 60.30(15) ?
O10 Bi7 Ba4 2_666 . 53.46(15) ?
O10 Bi7 Ba4 . . 126.54(15) ?
Ba4 Bi7 Ba4 2_666 . 180.0 ?
O5 Bi7 Ba1 . 2_666 122.5(2) ?
O5 Bi7 Ba1 2_666 2_666 57.5(2) ?
O11 Bi7 Ba1 2_666 2_666 120.62(15) ?
O11 Bi7 Ba1 . 2_666 59.38(15) ?
O10 Bi7 Ba1 2_666 2_666 48.84(16) ?
O10 Bi7 Ba1 . 2_666 131.16(16) ?
Ba4 Bi7 Ba1 2_666 2_666 109.605(10) ?
Ba4 Bi7 Ba1 . 2_666 70.395(10) ?
O5 Bi7 Ba1 . . 57.5(2) ?
O5 Bi7 Ba1 2_666 . 122.5(2) ?
O11 Bi7 Ba1 2_666 . 59.38(15) ?
O11 Bi7 Ba1 . . 120.62(15) ?
O10 Bi7 Ba1 2_666 . 131.16(16) ?
O10 Bi7 Ba1 . . 48.84(16) ?
Ba4 Bi7 Ba1 2_666 . 70.395(10) ?
Ba4 Bi7 Ba1 . . 109.604(10) ?
Ba1 Bi7 Ba1 2_666 . 180.000(16) ?
O5 Bi7 Ba3 . . 53.4(2) ?
O5 Bi7 Ba3 2_666 . 126.6(2) ?
O11 Bi7 Ba3 2_666 . 49.39(16) ?
O11 Bi7 Ba3 . . 130.61(16) ?
O10 Bi7 Ba3 2_666 . 60.63(16) ?
O10 Bi7 Ba3 . . 119.37(16) ?
Ba4 Bi7 Ba3 2_666 . 109.427(9) ?
Ba4 Bi7 Ba3 . . 70.572(9) ?
Ba1 Bi7 Ba3 2_666 . 109.454(11) ?
Ba1 Bi7 Ba3 . . 70.547(11) ?
O5 Bi7 Ba3 . 2_666 126.6(2) ?
O5 Bi7 Ba3 2_666 2_666 53.4(2) ?
O11 Bi7 Ba3 2_666 2_666 130.61(16) ?
O11 Bi7 Ba3 . 2_666 49.39(16) ?
O10 Bi7 Ba3 2_666 2_666 119.36(16) ?
O10 Bi7 Ba3 . 2_666 60.64(16) ?
Ba4 Bi7 Ba3 2_666 2_666 70.573(9) ?
Ba4 Bi7 Ba3 . 2_666 109.428(9) ?
Ba1 Bi7 Ba3 2_666 2_666 70.546(11) ?
Ba1 Bi7 Ba3 . 2_666 109.454(11) ?
Ba3 Bi7 Ba3 . 2_666 180.0 ?
O6 Bi8 O6 . 2 180.0 ?
O6 Bi8 O9 . 2_655 88.1(2) ?
O6 Bi8 O9 2 2_655 91.9(2) ?
O6 Bi8 O9 . 1_455 91.9(2) ?
O6 Bi8 O9 2 1_455 88.1(2) ?
O9 Bi8 O9 2_655 1_455 180.0(5) ?
O6 Bi8 O12 . 2_565 89.37(19) ?
O6 Bi8 O12 2 2_565 90.63(19) ?
O9 Bi8 O12 2_655 2_565 89.10(19) ?
O9 Bi8 O12 1_455 2_565 90.90(19) ?
O6 Bi8 O12 . 1_545 90.63(19) ?
O6 Bi8 O12 2 1_545 89.37(19) ?
O9 Bi8 O12 2_655 1_545 90.90(19) ?
O9 Bi8 O12 1_455 1_545 89.10(19) ?
O12 Bi8 O12 2_565 1_545 180.00(4) ?
O6 Bi8 Ba2 . . 58.33(17) ?
O6 Bi8 Ba2 2 . 121.67(17) ?
O9 Bi8 Ba2 2_655 . 130.88(17) ?
O9 Bi8 Ba2 1_455 . 49.12(17) ?
O12 Bi8 Ba2 2_565 . 58.81(14) ?
O12 Bi8 Ba2 1_545 . 121.19(14) ?
O6 Bi8 Ba2 . 2 121.67(17) ?
O6 Bi8 Ba2 2 2 58.33(17) ?
O9 Bi8 Ba2 2_655 2 49.12(17) ?
O9 Bi8 Ba2 1_455 2 130.88(17) ?
O12 Bi8 Ba2 2_565 2 121.19(14) ?
O12 Bi8 Ba2 1_545 2 58.81(14) ?
Ba2 Bi8 Ba2 . 2 180.0 ?
O6 Bi8 Ba3 . 1_544 51.35(17) ?
O6 Bi8 Ba3 2 1_544 128.65(17) ?
O9 Bi8 Ba3 2_655 1_544 52.68(15) ?
O9 Bi8 Ba3 1_455 1_544 127.32(15) ?
O12 Bi8 Ba3 2_565 1_544 120.00(15) ?
O12 Bi8 Ba3 1_545 1_544 60.00(15) ?
Ba2 Bi8 Ba3 . 1_544 109.608(10) ?
Ba2 Bi8 Ba3 2 1_544 70.392(10) ?
O6 Bi8 Ba3 . 2_566 128.65(17) ?
O6 Bi8 Ba3 2 2_566 51.35(17) ?
O9 Bi8 Ba3 2_655 2_566 127.32(15) ?
O9 Bi8 Ba3 1_455 2_566 52.68(15) ?
O12 Bi8 Ba3 2_565 2_566 60.00(15) ?
O12 Bi8 Ba3 1_545 2_566 120.00(15) ?
Ba2 Bi8 Ba3 . 2_566 70.392(10) ?
Ba2 Bi8 Ba3 2 2_566 109.608(10) ?
Ba3 Bi8 Ba3 1_544 2_566 180.000(15) ?
O6 Bi8 Ba4 . 1_554 52.31(17) ?
O6 Bi8 Ba4 2 1_554 127.69(17) ?
O9 Bi8 Ba4 2_655 1_554 60.33(17) ?
O9 Bi8 Ba4 1_455 1_554 119.67(17) ?
O12 Bi8 Ba4 2_565 1_554 49.71(15) ?
O12 Bi8 Ba4 1_545 1_554 130.29(15) ?
Ba2 Bi8 Ba4 . 1_554 70.603(11) ?
Ba2 Bi8 Ba4 2 1_554 109.397(11) ?
Ba3 Bi8 Ba4 1_544 1_554 70.481(9) ?
Ba3 Bi8 Ba4 2_566 1_554 109.519(9) ?
O6 Bi8 Ba4 . 2_556 127.69(17) ?
O6 Bi8 Ba4 2 2_556 52.31(17) ?
O9 Bi8 Ba4 2_655 2_556 119.67(17) ?
O9 Bi8 Ba4 1_455 2_556 60.33(17) ?
O12 Bi8 Ba4 2_565 2_556 130.29(15) ?
O12 Bi8 Ba4 1_545 2_556 49.71(15) ?
Ba2 Bi8 Ba4 . 2_556 109.397(11) ?
Ba2 Bi8 Ba4 2 2_556 70.603(11) ?
Ba3 Bi8 Ba4 1_544 2_556 109.519(9) ?
Ba3 Bi8 Ba4 2_566 2_556 70.481(9) ?
Ba4 Bi8 Ba4 1_554 2_556 180.0 ?
O1 Bi5 O1 2_666 1_545 180.0 ?
O1 Bi5 O7 2_666 2_666 88.9(2) ?
O1 Bi5 O7 1_545 2_666 91.1(2) ?
O1 Bi5 O7 2_666 1_545 91.1(2) ?
O1 Bi5 O7 1_545 1_545 88.9(2) ?
O7 Bi5 O7 2_666 1_545 180.0 ?
O1 Bi5 O11 2_666 . 92.09(19) ?
O1 Bi5 O11 1_545 . 87.91(19) ?
O7 Bi5 O11 2_666 . 90.70(19) ?
O7 Bi5 O11 1_545 . 89.30(19) ?
O1 Bi5 O11 2_666 2_656 87.91(19) ?
O1 Bi5 O11 1_545 2_656 92.09(19) ?
O7 Bi5 O11 2_666 2_656 89.30(19) ?
O7 Bi5 O11 1_545 2_656 90.70(19) ?
O11 Bi5 O11 . 2_656 180.0 ?
O1 Bi5 Ba1 2_666 2_666 53.43(15) ?
O1 Bi5 Ba1 1_545 2_666 126.57(15) ?
O7 Bi5 Ba1 2_666 2_666 52.38(16) ?
O7 Bi5 Ba1 1_545 2_666 127.62(16) ?
O11 Bi5 Ba1 . 2_666 59.61(15) ?
O11 Bi5 Ba1 2_656 2_666 120.39(15) ?
O1 Bi5 Ba1 2_666 1_545 126.57(15) ?
O1 Bi5 Ba1 1_545 1_545 53.43(15) ?
O7 Bi5 Ba1 2_666 1_545 127.62(16) ?
O7 Bi5 Ba1 1_545 1_545 52.38(16) ?
O11 Bi5 Ba1 . 1_545 120.39(15) ?
O11 Bi5 Ba1 2_656 1_545 59.61(15) ?
Ba1 Bi5 Ba1 2_666 1_545 180.0 ?
O1 Bi5 Ba4 2_666 2_656 131.06(17) ?
O1 Bi5 Ba4 1_545 2_656 48.94(17) ?
O7 Bi5 Ba4 2_666 2_656 57.21(16) ?
O7 Bi5 Ba4 1_545 2_656 122.79(16) ?
O11 Bi5 Ba4 . 2_656 119.56(15) ?
O11 Bi5 Ba4 2_656 2_656 60.44(15) ?
Ba1 Bi5 Ba4 2_666 2_656 109.440(10) ?
Ba1 Bi5 Ba4 1_545 2_656 70.560(10) ?
O1 Bi5 Ba4 2_666 . 48.94(17) ?
O1 Bi5 Ba4 1_545 . 131.06(17) ?
O7 Bi5 Ba4 2_666 . 122.79(16) ?
O7 Bi5 Ba4 1_545 . 57.21(16) ?
O11 Bi5 Ba4 . . 60.44(15) ?
O11 Bi5 Ba4 2_656 . 119.56(15) ?
Ba1 Bi5 Ba4 2_666 . 70.560(10) ?
Ba1 Bi5 Ba4 1_545 . 109.440(10) ?
Ba4 Bi5 Ba4 2_656 . 180.0 ?
O1 Bi5 Ba3 2_666 1_545 56.40(15) ?
O1 Bi5 Ba3 1_545 1_545 123.60(15) ?
O7 Bi5 Ba3 2_666 1_545 121.57(17) ?
O7 Bi5 Ba3 1_545 1_545 58.43(17) ?
O11 Bi5 Ba3 . 1_545 130.73(16) ?
O11 Bi5 Ba3 2_656 1_545 49.27(16) ?
Ba1 Bi5 Ba3 2_666 1_545 109.397(12) ?
Ba1 Bi5 Ba3 1_545 1_545 70.603(12) ?
Ba4 Bi5 Ba3 2_656 1_545 109.440(9) ?
Ba4 Bi5 Ba3 . 1_545 70.560(8) ?
O1 Bi5 Ba3 2_666 2_666 123.60(15) ?
O1 Bi5 Ba3 1_545 2_666 56.40(15) ?
O7 Bi5 Ba3 2_666 2_666 58.43(17) ?
O7 Bi5 Ba3 1_545 2_666 121.57(17) ?
O11 Bi5 Ba3 . 2_666 49.27(16) ?
O11 Bi5 Ba3 2_656 2_666 130.73(16) ?
Ba1 Bi5 Ba3 2_666 2_666 70.603(12) ?
Ba1 Bi5 Ba3 1_545 2_666 109.397(12) ?
Ba4 Bi5 Ba3 2_656 2_666 70.560(8) ?
Ba4 Bi5 Ba3 . 2_666 109.440(8) ?
Ba3 Bi5 Ba3 1_545 2_666 180.0 ?
O2 Bi6 O2 2_565 . 180.0 ?
O2 Bi6 O8 2_565 2_565 90.3(2) ?
O2 Bi6 O8 . 2_565 89.7(2) ?
O2 Bi6 O8 2_565 . 89.7(2) ?
O2 Bi6 O8 . . 90.3(2) ?
O8 Bi6 O8 2_565 . 180.0 ?
O2 Bi6 O12 2_565 . 91.83(19) ?
O2 Bi6 O12 . . 88.17(19) ?
O8 Bi6 O12 2_565 . 90.2(2) ?
O8 Bi6 O12 . . 89.8(2) ?
O2 Bi6 O12 2_565 2_565 88.17(19) ?
O2 Bi6 O12 . 2_565 91.83(19) ?
O8 Bi6 O12 2_565 2_565 89.8(2) ?
O8 Bi6 O12 . 2_565 90.2(2) ?
O12 Bi6 O12 . 2_565 180.0 ?
O2 Bi6 Ba2 2_565 2_565 53.39(15) ?
O2 Bi6 Ba2 . 2_565 126.61(15) ?
O8 Bi6 Ba2 2_565 2_565 53.6(2) ?
O8 Bi6 Ba2 . 2_565 126.4(2) ?
O12 Bi6 Ba2 . 2_565 58.99(14) ?
O12 Bi6 Ba2 2_565 2_565 121.01(14) ?
O2 Bi6 Ba2 2_565 . 126.61(15) ?
O2 Bi6 Ba2 . . 53.39(15) ?
O8 Bi6 Ba2 2_565 . 126.4(2) ?
O8 Bi6 Ba2 . . 53.6(2) ?
O12 Bi6 Ba2 . . 121.02(14) ?
O12 Bi6 Ba2 2_565 . 58.98(14) ?
Ba2 Bi6 Ba2 2_565 . 180.0 ?
O2 Bi6 Ba3 2_565 1_554 49.39(16) ?
O2 Bi6 Ba3 . 1_554 130.61(16) ?
O8 Bi6 Ba3 2_565 1_554 124.1(2) ?
O8 Bi6 Ba3 . 1_554 55.9(2) ?
O12 Bi6 Ba3 . 1_554 60.18(15) ?
O12 Bi6 Ba3 2_565 1_554 119.82(15) ?
Ba2 Bi6 Ba3 2_565 1_554 70.533(10) ?
Ba2 Bi6 Ba3 . 1_554 109.467(10) ?
O2 Bi6 Ba3 2_565 2_566 130.61(16) ?
O2 Bi6 Ba3 . 2_566 49.39(16) ?
O8 Bi6 Ba3 2_565 2_566 55.9(2) ?
O8 Bi6 Ba3 . 2_566 124.1(2) ?
O12 Bi6 Ba3 . 2_566 119.82(15) ?
O12 Bi6 Ba3 2_565 2_566 60.18(15) ?
Ba2 Bi6 Ba3 2_565 2_566 109.467(10) ?
Ba2 Bi6 Ba3 . 2_566 70.533(10) ?
Ba3 Bi6 Ba3 1_554 2_566 180.0 ?
O2 Bi6 Ba4 2_565 1_554 56.37(15) ?
O2 Bi6 Ba4 . 1_554 123.63(15) ?
O8 Bi6 Ba4 2_565 1_554 122.8(2) ?
O8 Bi6 Ba4 . 1_554 57.2(2) ?
O12 Bi6 Ba4 . 1_554 130.47(15) ?
O12 Bi6 Ba4 2_565 1_554 49.53(15) ?
Ba2 Bi6 Ba4 2_565 1_554 109.401(12) ?
Ba2 Bi6 Ba4 . 1_554 70.599(12) ?
Ba3 Bi6 Ba4 1_554 1_554 70.494(8) ?
Ba3 Bi6 Ba4 2_566 1_554 109.506(8) ?
O2 Bi6 Ba4 2_565 2_566 123.63(15) ?
O2 Bi6 Ba4 . 2_566 56.37(15) ?
O8 Bi6 Ba4 2_565 2_566 57.2(2) ?
O8 Bi6 Ba4 . 2_566 122.8(2) ?
O12 Bi6 Ba4 . 2_566 49.53(15) ?
O12 Bi6 Ba4 2_565 2_566 130.47(15) ?
Ba2 Bi6 Ba4 2_565 2_566 70.599(12) ?
Ba2 Bi6 Ba4 . 2_566 109.401(12) ?
Ba3 Bi6 Ba4 1_554 2_566 109.506(8) ?
Ba3 Bi6 Ba4 2_566 2_566 70.494(8) ?
Ba4 Bi6 Ba4 1_554 2_566 180.000(12) ?
O10 Ba1 O3 . 2_566 124.93(15) ?
O10 Ba1 O12 . . 122.48(16) ?
O3 Ba1 O12 2_566 . 82.87(14) ?
O10 Ba1 O7 . . 121.20(15) ?
O3 Ba1 O7 2_566 . 60.70(16) ?
O12 Ba1 O7 . . 116.32(17) ?
O10 Ba1 O8 . . 60.41(16) ?
O3 Ba1 O8 2_566 . 119.46(18) ?
O12 Ba1 O8 . . 62.09(19) ?
O7 Ba1 O8 . . 178.13(17) ?
O10 Ba1 O1 . . 85.07(15) ?
O3 Ba1 O1 2_566 . 119.50(15) ?
O12 Ba1 O1 . . 127.31(17) ?
O7 Ba1 O1 . . 58.9(2) ?
O8 Ba1 O1 . . 121.0(2) ?
O10 Ba1 O6 . 1_565 120.29(19) ?
O3 Ba1 O6 2_566 1_565 114.65(16) ?
O12 Ba1 O6 . 1_565 58.82(17) ?
O7 Ba1 O6 . 1_565 89.78(15) ?
O8 Ba1 O6 . 1_565 88.51(18) ?
O1 Ba1 O6 . 1_565 68.53(13) ?
O10 Ba1 O9 . 1_465 175.26(15) ?
O3 Ba1 O9 2_566 1_465 58.20(15) ?
O12 Ba1 O9 . 1_465 60.29(16) ?
O7 Ba1 O9 . 1_465 56.24(14) ?
O8 Ba1 O9 . 1_465 122.08(16) ?
O1 Ba1 O9 . 1_465 90.22(16) ?
O6 Ba1 O9 1_565 1_465 57.02(17) ?
O10 Ba1 O5 . . 59.2(2) ?
O3 Ba1 O5 2_566 . 65.73(17) ?
O12 Ba1 O5 . . 119.75(19) ?
O7 Ba1 O5 . . 91.90(18) ?
O8 Ba1 O5 . . 89.80(16) ?
O1 Ba1 O5 . . 112.94(15) ?
O6 Ba1 O5 1_565 . 178.20(16) ?
O9 Ba1 O5 1_465 . 123.59(19) ?
O10 Ba1 O11 . 2_666 61.88(16) ?
O3 Ba1 O11 2_566 2_666 89.28(16) ?
O12 Ba1 O11 . 2_666 172.10(18) ?
O7 Ba1 O11 . 2_666 59.70(15) ?
O8 Ba1 O11 . 2_666 122.0(2) ?
O1 Ba1 O11 . 2_666 57.74(16) ?
O6 Ba1 O11 1_565 2_666 126.06(18) ?
O9 Ba1 O11 1_465 2_666 115.89(15) ?
O5 Ba1 O11 . 2_666 55.50(17) ?
O10 Ba1 O4 . 1_554 58.61(14) ?
O3 Ba1 O4 2_566 1_554 174.23(17) ?
O12 Ba1 O4 . 1_554 91.37(15) ?
O7 Ba1 O4 . 1_554 122.43(16) ?
O8 Ba1 O4 . 1_554 57.23(16) ?
O1 Ba1 O4 . 1_554 64.13(15) ?
O6 Ba1 O4 1_565 1_554 61.68(14) ?
O9 Ba1 O4 1_465 1_554 118.61(13) ?
O5 Ba1 O4 . 1_554 117.79(18) ?
O11 Ba1 O4 2_666 1_554 96.49(13) ?
O10 Ba1 O2 . . 90.06(13) ?
O3 Ba1 O2 2_566 . 63.42(14) ?
O12 Ba1 O2 . . 55.90(16) ?
O7 Ba1 O2 . . 124.11(18) ?
O8 Ba1 O2 . . 56.12(19) ?
O1 Ba1 O2 . . 175.12(13) ?
O6 Ba1 O2 1_565 . 114.38(13) ?
O9 Ba1 O2 1_465 . 94.65(14) ?
O5 Ba1 O2 . . 64.09(14) ?
O11 Ba1 O2 2_666 . 119.56(15) ?
O4 Ba1 O2 1_554 . 113.32(13) ?
O9 Ba2 O4 1_455 2_666 125.05(16) ?
O9 Ba2 O11 1_455 . 123.06(17) ?
O4 Ba2 O11 2_666 . 82.84(14) ?
O9 Ba2 O7 1_455 1_545 59.94(15) ?
O4 Ba2 O7 2_666 1_545 119.45(17) ?
O11 Ba2 O7 . 1_545 63.12(17) ?
O9 Ba2 O2 1_455 . 84.90(15) ?
O4 Ba2 O2 2_666 . 119.34(14) ?
O11 Ba2 O2 . . 126.96(16) ?
O7 Ba2 O2 1_545 . 121.17(19) ?
O9 Ba2 O8 1_455 . 119.85(16) ?
O4 Ba2 O8 2_666 . 60.63(17) ?
O11 Ba2 O8 . . 117.1(2) ?
O7 Ba2 O8 1_545 . 179.80(17) ?
O2 Ba2 O8 . . 58.7(2) ?
O9 Ba2 O5 1_455 . 120.2(2) ?
O4 Ba2 O5 2_666 . 114.73(18) ?
O11 Ba2 O5 . . 59.34(19) ?
O7 Ba2 O5 1_545 . 89.90(19) ?
O2 Ba2 O5 . . 67.67(15) ?
O8 Ba2 O5 . . 90.22(17) ?
O9 Ba2 O10 1_455 . 174.49(16) ?
O4 Ba2 O10 2_666 . 58.35(14) ?
O11 Ba2 O10 . . 60.39(17) ?
O7 Ba2 O10 1_545 . 123.23(13) ?
O2 Ba2 O10 . . 89.60(15) ?
O8 Ba2 O10 . . 56.97(16) ?
O5 Ba2 O10 . . 56.91(19) ?
O9 Ba2 O6 1_455 . 59.61(19) ?
O4 Ba2 O6 2_666 . 65.49(15) ?
O11 Ba2 O6 . . 120.37(17) ?
O7 Ba2 O6 1_545 . 89.62(14) ?
O2 Ba2 O6 . . 112.63(13) ?
O8 Ba2 O6 . . 90.26(18) ?
O5 Ba2 O6 . . 179.52(18) ?
O10 Ba2 O6 . . 123.37(17) ?
O9 Ba2 O12 1_455 2_565 61.39(17) ?
O4 Ba2 O12 2_666 2_565 89.47(16) ?
O11 Ba2 O12 . 2_565 172.29(18) ?
O7 Ba2 O12 1_545 2_565 121.00(18) ?
O2 Ba2 O12 . 2_565 57.78(16) ?
O8 Ba2 O12 . 2_565 58.80(18) ?
O5 Ba2 O12 . 2_565 125.3(2) ?
O10 Ba2 O12 . 2_565 115.75(16) ?
O6 Ba2 O12 . 2_565 55.06(15) ?
O9 Ba2 O3 1_455 . 58.58(14) ?
O4 Ba2 O3 2_666 . 174.14(17) ?
O11 Ba2 O3 . . 91.30(16) ?
O7 Ba2 O3 1_545 . 57.27(14) ?
O2 Ba2 O3 . . 64.33(15) ?
O8 Ba2 O3 . . 122.66(18) ?
O5 Ba2 O3 . . 61.62(16) ?
O10 Ba2 O3 . . 118.46(13) ?
O6 Ba2 O3 . . 118.12(15) ?
O12 Ba2 O3 2_565 . 96.39(13) ?
O9 Ba2 O1 1_455 1_545 90.67(13) ?
O4 Ba2 O1 2_666 1_545 63.48(13) ?
O11 Ba2 O1 . 1_545 55.79(16) ?
O7 Ba2 O1 1_545 1_545 56.00(18) ?
O2 Ba2 O1 . 1_545 175.58(13) ?
O8 Ba2 O1 . 1_545 124.08(19) ?
O5 Ba2 O1 . 1_545 114.79(15) ?
O10 Ba2 O1 . 1_545 94.82(14) ?
O6 Ba2 O1 . 1_545 64.88(12) ?
O12 Ba2 O1 2_565 1_545 119.93(15) ?
O3 Ba2 O1 . 1_545 113.17(14) ?
O11 Ba3 O2 2_666 2_566 125.29(17) ?
O11 Ba3 O4 2_666 . 82.76(14) ?
O2 Ba3 O4 2_566 . 118.02(14) ?
O11 Ba3 O6 2_666 1_566 119.27(19) ?
O2 Ba3 O6 2_566 1_566 115.43(15) ?
O4 Ba3 O6 . 1_566 67.92(15) ?
O11 Ba3 O9 2_666 2_666 124.40(17) ?
O2 Ba3 O9 2_566 2_666 84.82(15) ?
O4 Ba3 O9 . 2_666 126.78(14) ?
O6 Ba3 O9 1_566 2_666 58.89(19) ?
O11 Ba3 O5 2_666 . 60.84(18) ?
O2 Ba3 O5 2_566 . 64.46(16) ?
O4 Ba3 O5 . . 112.39(19) ?
O6 Ba3 O5 1_566 . 179.69(16) ?
O9 Ba3 O5 2_666 . 120.8(2) ?
O11 Ba3 O8 2_666 1_556 119.2(2) ?
O2 Ba3 O8 2_566 1_556 58.7(2) ?
O4 Ba3 O8 . 1_556 59.44(16) ?
O6 Ba3 O8 1_566 1_556 90.15(18) ?
O9 Ba3 O8 2_666 1_556 116.39(16) ?
O5 Ba3 O8 . 1_556 90.03(17) ?
O11 Ba3 O1 2_666 2_676 58.07(16) ?
O2 Ba3 O1 2_566 2_676 175.05(14) ?
O4 Ba3 O1 . 2_676 65.02(14) ?
O6 Ba3 O1 1_566 2_676 61.41(14) ?
O9 Ba3 O1 2_666 2_676 90.23(16) ?
O5 Ba3 O1 . 2_676 118.67(15) ?
O8 Ba3 O1 1_556 2_676 123.89(19) ?
O11 Ba3 O7 2_666 . 61.06(16) ?
O2 Ba3 O7 2_566 . 121.01(18) ?
O4 Ba3 O7 . . 120.86(15) ?
O6 Ba3 O7 1_566 . 89.85(14) ?
O9 Ba3 O7 2_666 . 63.34(14) ?
O5 Ba3 O7 . . 89.97(18) ?
O8 Ba3 O7 1_556 . 179.67(15) ?
O1 Ba3 O7 2_676 . 56.38(17) ?
O11 Ba3 O3 2_666 2_566 90.05(16) ?
O2 Ba3 O3 2_566 2_566 66.32(15) ?
O4 Ba3 O3 . 2_566 172.81(17) ?
O6 Ba3 O3 1_566 2_566 116.20(16) ?
O9 Ba3 O3 2_666 2_566 57.90(15) ?
O5 Ba3 O3 . 2_566 63.49(17) ?
O8 Ba3 O3 1_556 2_566 124.98(18) ?
O1 Ba3 O3 2_676 2_566 111.10(14) ?
O7 Ba3 O3 . 2_566 54.74(14) ?
O11 Ba3 O12 2_666 1_556 173.69(18) ?
O2 Ba3 O12 2_566 1_556 58.35(16) ?
O4 Ba3 O12 . 1_556 90.94(15) ?
O6 Ba3 O12 1_566 1_556 57.31(16) ?
O9 Ba3 O12 2_666 1_556 59.46(16) ?
O5 Ba3 O12 . 1_556 122.61(19) ?
O8 Ba3 O12 1_556 1_556 57.12(18) ?
O1 Ba3 O12 2_676 1_556 118.71(15) ?
O7 Ba3 O12 . 1_556 122.63(16) ?
O3 Ba3 O12 2_566 1_556 96.25(13) ?
O11 Ba3 O10 2_666 2_666 58.87(16) ?
O2 Ba3 O10 2_566 2_666 90.11(13) ?
O4 Ba3 O10 . 2_666 56.07(13) ?
O6 Ba3 O10 1_566 2_666 123.93(17) ?
O9 Ba3 O10 2_666 2_666 174.92(15) ?
O5 Ba3 O10 . 2_666 56.38(19) ?
O8 Ba3 O10 1_556 2_666 60.58(16) ?
O1 Ba3 O10 2_676 2_666 94.84(14) ?
O7 Ba3 O10 . 2_666 119.67(14) ?
O3 Ba3 O10 2_566 2_666 119.77(12) ?
O12 Ba3 O10 1_556 2_666 117.70(15) ?
O1 Ba4 O12 2_666 2_566 124.90(17) ?
O1 Ba4 O3 2_666 . 118.20(14) ?
O12 Ba4 O3 2_566 . 83.14(14) ?
O1 Ba4 O5 2_666 . 115.39(16) ?
O12 Ba4 O5 2_566 . 119.7(2) ?
O3 Ba4 O5 . . 67.46(18) ?
O1 Ba4 O6 2_666 1_556 64.24(15) ?
O12 Ba4 O6 2_566 1_556 60.65(17) ?
O3 Ba4 O6 . 1_556 111.72(17) ?
O5 Ba4 O6 . 1_556 178.91(17) ?
O1 Ba4 O10 2_666 2_666 84.72(15) ?
O12 Ba4 O10 2_566 2_666 123.72(17) ?
O3 Ba4 O10 . 2_666 127.39(14) ?
O5 Ba4 O10 . 2_666 59.9(2) ?
O6 Ba4 O10 1_556 2_666 120.85(19) ?
O1 Ba4 O2 2_666 2_566 175.42(13) ?
O12 Ba4 O2 2_566 2_566 57.93(17) ?
O3 Ba4 O2 . 2_566 64.86(14) ?
O5 Ba4 O2 . 2_566 61.99(16) ?
O6 Ba4 O2 1_556 2_566 118.45(13) ?
O10 Ba4 O2 2_666 2_566 90.70(15) ?
O1 Ba4 O7 2_666 1_545 59.57(18) ?
O12 Ba4 O7 2_566 1_545 119.75(18) ?
O3 Ba4 O7 . 1_545 58.82(14) ?
O5 Ba4 O7 . 1_545 88.63(18) ?
O6 Ba4 O7 1_556 1_545 90.31(15) ?
O10 Ba4 O7 2_666 1_545 116.53(14) ?
O2 Ba4 O7 2_566 1_545 123.06(17) ?
O1 Ba4 O8 2_666 1_556 121.7(2) ?
O12 Ba4 O8 2_566 1_556 60.72(17) ?
O3 Ba4 O8 . 1_556 120.04(18) ?
O5 Ba4 O8 . 1_556 89.81(16) ?
O6 Ba4 O8 1_556 1_556 91.24(18) ?
O10 Ba4 O8 2_666 1_556 63.00(16) ?
O2 Ba4 O8 2_566 1_556 55.64(19) ?
O7 Ba4 O8 1_545 1_556 178.36(16) ?
O1 Ba4 O4 2_666 2_667 66.15(14) ?
O12 Ba4 O4 2_566 2_667 89.47(16) ?
O3 Ba4 O4 . 2_667 172.61(17) ?
O5 Ba4 O4 . 2_667 116.92(18) ?
O6 Ba4 O4 1_556 2_667 63.98(14) ?
O10 Ba4 O4 2_666 2_667 57.48(14) ?
O2 Ba4 O4 2_566 2_667 111.21(13) ?
O7 Ba4 O4 1_545 2_667 125.69(15) ?
O8 Ba4 O4 1_556 2_667 55.58(16) ?
O1 Ba4 O11 2_666 . 58.66(16) ?
O12 Ba4 O11 2_566 . 174.07(17) ?
O3 Ba4 O11 . . 90.95(16) ?
O5 Ba4 O11 . . 56.90(19) ?
O6 Ba4 O11 1_556 . 122.64(17) ?
O10 Ba4 O11 2_666 . 59.85(15) ?
O2 Ba4 O11 2_566 . 118.89(16) ?
O7 Ba4 O11 1_545 . 56.85(16) ?
O8 Ba4 O11 1_556 . 122.53(18) ?
O4 Ba4 O11 2_667 . 96.43(13) ?
O1 Ba4 O9 2_666 2_656 89.65(13) ?
O12 Ba4 O9 2_566 2_656 59.24(16) ?
O3 Ba4 O9 . 2_656 56.48(13) ?
O5 Ba4 O9 . 2_656 123.83(19) ?
O6 Ba4 O9 1_556 2_656 55.31(17) ?
O10 Ba4 O9 2_666 2_656 174.29(15) ?
O2 Ba4 O9 2_566 2_656 94.93(14) ?
O7 Ba4 O9 1_545 2_656 60.86(14) ?
O8 Ba4 O9 1_556 2_656 119.76(15) ?
O4 Ba4 O9 2_667 2_656 119.19(13) ?
O11 Ba4 O9 . 2_656 117.70(15) ?
Bi5 O1 Na2 1_565 1_565 168.7(3) ?
Bi5 O1 Ba4 1_565 2_666 98.9(2) ?
Na2 O1 Ba4 1_565 2_666 92.1(2) ?
Bi5 O1 Ba1 1_565 . 94.0(2) ?
Na2 O1 Ba1 1_565 . 87.91(17) ?
Ba4 O1 Ba1 2_666 . 94.85(15) ?
Bi5 O1 Ba3 1_565 2_676 91.10(18) ?
Na2 O1 Ba3 1_565 2_676 85.50(17) ?
Ba4 O1 Ba3 2_666 2_676 92.59(17) ?
Ba1 O1 Ba3 . 2_676 170.2(2) ?
Bi5 O1 Ba2 1_565 1_565 87.0(2) ?
Na2 O1 Ba2 1_565 1_565 81.94(17) ?
Ba4 O1 Ba2 2_666 1_565 173.8(2) ?
Ba1 O1 Ba2 . 1_565 86.79(15) ?
Ba3 O1 Ba2 2_676 1_565 85.16(12) ?
Bi6 O2 Bi1 . . 169.6(3) ?
Bi6 O2 Ba3 . 2_566 98.4(2) ?
Bi1 O2 Ba3 . 2_566 91.4(2) ?
Bi6 O2 Ba2 . . 94.1(2) ?
Bi1 O2 Ba2 . . 88.21(17) ?
Ba3 O2 Ba2 2_566 . 94.51(14) ?
Bi6 O2 Ba4 . 2_566 91.22(18) ?
Bi1 O2 Ba4 . 2_566 85.28(17) ?
Ba3 O2 Ba4 2_566 2_566 92.21(16) ?
Ba2 O2 Ba4 . 2_566 170.8(2) ?
Bi6 O2 Ba1 . . 87.49(19) ?
Bi1 O2 Ba1 . . 82.53(16) ?
Ba3 O2 Ba1 2_566 . 173.7(2) ?
Ba2 O2 Ba1 . . 87.25(15) ?
Ba4 O2 Ba1 2_566 . 85.41(12) ?
Bi3 O3 Bi1 . . 167.1(2) ?
Bi3 O3 Ba1 . 2_566 98.1(2) ?
Bi1 O3 Ba1 . 2_566 91.65(16) ?
Bi3 O3 Ba4 . . 96.70(19) ?
Bi1 O3 Ba4 . . 90.46(15) ?
Ba1 O3 Ba4 2_566 . 96.89(13) ?
Bi3 O3 Ba3 . 2_566 88.26(15) ?
Bi1 O3 Ba3 . 2_566 83.26(14) ?
Ba1 O3 Ba3 2_566 2_566 90.22(17) ?
Ba4 O3 Ba3 . 2_566 170.7(2) ?
Bi3 O3 Ba2 . . 87.12(17) ?
Bi1 O3 Ba2 . . 82.32(15) ?
Ba1 O3 Ba2 2_566 . 171.78(18) ?
Ba4 O3 Ba2 . . 88.77(17) ?
Ba3 O3 Ba2 2_566 . 83.55(10) ?
Na4 O4 Na2 1_556 1_566 167.6(2) ?
Na4 O4 Ba2 1_556 2_666 97.88(19) ?
Na2 O4 Ba2 1_566 2_666 91.58(16) ?
Na4 O4 Ba3 1_556 . 96.45(18) ?
Na2 O4 Ba3 1_566 . 90.34(15) ?
Ba2 O4 Ba3 2_666 . 96.58(13) ?
Na4 O4 Ba4 1_556 2_667 88.44(15) ?
Na2 O4 Ba4 1_566 2_667 83.52(14) ?
Ba2 O4 Ba4 2_666 2_667 90.30(17) ?
Ba3 O4 Ba4 . 2_667 170.91(19) ?
Na4 O4 Ba1 1_556 1_556 87.33(16) ?
Na2 O4 Ba1 1_566 1_556 82.46(14) ?
Ba2 O4 Ba1 2_666 1_556 172.01(18) ?
Ba3 O4 Ba1 . 1_556 88.81(17) ?
Ba4 O4 Ba1 2_667 1_556 83.76(10) ?
Bi7 O5 Bi1 . . 174.6(4) ?
Bi7 O5 Ba4 . . 95.2(3) ?
Bi1 O5 Ba4 . . 89.6(2) ?
Bi7 O5 Ba3 . . 93.9(3) ?
Bi1 O5 Ba3 . . 88.4(2) ?
Ba4 O5 Ba3 . . 92.6(2) ?
Bi7 O5 Ba2 . . 91.3(3) ?
Bi1 O5 Ba2 . . 86.1(2) ?
Ba4 O5 Ba2 . . 90.7(2) ?
Ba3 O5 Ba2 . . 173.6(3) ?
Bi7 O5 Ba1 . . 89.8(3) ?
Bi1 O5 Ba1 . . 85.4(2) ?
Ba4 O5 Ba1 . . 174.7(3) ?
Ba3 O5 Ba1 . . 88.9(2) ?
Ba2 O5 Ba1 . . 87.32(19) ?
Bi8 O6 Bi2 . . 172.0(3) ?
Bi8 O6 Ba3 . 1_544 96.4(2) ?
Bi2 O6 Ba3 . 1_544 90.0(2) ?
Bi8 O6 Ba4 . 1_554 95.4(2) ?
Bi2 O6 Ba4 . 1_554 89.1(2) ?
Ba3 O6 Ba4 1_544 1_554 93.79(17) ?
Bi8 O6 Ba1 . 1_545 90.3(2) ?
Bi2 O6 Ba1 . 1_545 84.68(19) ?
Ba3 O6 Ba1 1_544 1_545 90.40(16) ?
Ba4 O6 Ba1 1_554 1_545 172.5(3) ?
Bi8 O6 Ba2 . . 89.1(2) ?
Bi2 O6 Ba2 . . 84.28(19) ?
Ba3 O6 Ba2 1_544 . 173.5(2) ?
Ba4 O6 Ba2 1_554 . 89.14(16) ?
Ba1 O6 Ba2 1_545 . 86.09(15) ?
Na3 O7 Bi5 1_565 1_565 171.2(3) ?
Na3 O7 Ba2 1_565 1_565 93.4(2) ?
Bi5 O7 Ba2 1_565 1_565 93.7(2) ?
Na3 O7 Ba1 1_565 . 92.5(2) ?
Bi5 O7 Ba1 1_565 . 92.1(2) ?
Ba2 O7 Ba1 1_565 . 94.38(18) ?
Na3 O7 Ba4 1_565 1_565 87.4(2) ?
Bi5 O7 Ba4 1_565 1_565 87.3(2) ?
Ba2 O7 Ba4 1_565 1_565 90.65(16) ?
Ba1 O7 Ba4 . 1_565 175.0(2) ?
Na3 O7 Ba3 1_565 . 86.3(2) ?
Bi5 O7 Ba3 1_565 . 86.3(2) ?
Ba2 O7 Ba3 1_565 . 176.5(2) ?
Ba1 O7 Ba3 . . 89.07(16) ?
Ba4 O7 Ba3 1_565 . 85.89(16) ?
Bi6 O8 Bi4 . . 174.9(4) ?
Bi6 O8 Ba1 . . 92.9(3) ?
Bi4 O8 Ba1 . . 91.6(2) ?
Bi6 O8 Ba2 . . 91.4(2) ?
Bi4 O8 Ba2 . . 90.8(3) ?
Ba1 O8 Ba2 . . 92.6(2) ?
Bi6 O8 Ba3 . 1_554 89.1(2) ?
Bi4 O8 Ba3 . 1_554 88.4(2) ?
Ba1 O8 Ba3 . 1_554 90.73(19) ?
Ba2 O8 Ba3 . 1_554 176.6(3) ?
Bi6 O8 Ba4 . 1_554 88.1(2) ?
Bi4 O8 Ba4 . 1_554 87.3(2) ?
Ba1 O8 Ba4 . 1_554 177.9(3) ?
Ba2 O8 Ba4 . 1_554 89.18(19) ?
Ba3 O8 Ba4 1_554 1_554 87.5(2) ?
Na8 O9 Na3 1_655 1_655 167.7(3) ?
Na8 O9 Ba2 1_655 1_655 95.6(2) ?
Na3 O9 Ba2 1_655 1_655 95.7(2) ?
Na8 O9 Ba3 1_655 2_666 91.92(19) ?
Na3 O9 Ba3 1_655 2_666 91.8(2) ?
Ba2 O9 Ba3 1_655 2_666 95.62(17) ?
Na8 O9 Ba1 1_655 1_645 87.48(19) ?
Na3 O9 Ba1 1_655 1_645 87.24(17) ?
Ba2 O9 Ba1 1_655 1_645 92.17(18) ?
Ba3 O9 Ba1 2_666 1_645 172.2(2) ?
Na8 O9 Ba4 1_655 2_656 84.46(18) ?
Na3 O9 Ba4 1_655 2_656 83.97(19) ?
Ba2 O9 Ba4 1_655 2_656 177.0(2) ?
Ba3 O9 Ba4 2_666 2_656 87.38(16) ?
Ba1 O9 Ba4 1_645 2_656 84.83(14) ?
Bi4 O10 Bi7 . . 167.7(3) ?
Bi4 O10 Ba1 . . 96.2(2) ?
Bi7 O10 Ba1 . . 95.7(2) ?
Bi4 O10 Ba4 . 2_666 91.59(19) ?
Bi7 O10 Ba4 . 2_666 90.83(18) ?
Ba1 O10 Ba4 . 2_666 95.23(16) ?
Bi4 O10 Ba2 . . 87.91(17) ?
Bi7 O10 Ba2 . . 87.97(18) ?
Ba1 O10 Ba2 . . 92.95(17) ?
Ba4 O10 Ba2 2_666 . 171.8(2) ?
Bi4 O10 Ba3 . 2_666 84.13(19) ?
Bi7 O10 Ba3 . 2_666 83.93(18) ?
Ba1 O10 Ba3 . 2_666 178.0(2) ?
Ba4 O10 Ba3 2_666 2_666 86.78(16) ?
Ba2 O10 Ba3 . 2_666 85.04(13) ?
Bi5 O11 Bi7 . . 165.5(2) ?
Bi5 O11 Ba3 . 2_666 95.5(2) ?
Bi7 O11 Ba3 . 2_666 95.1(2) ?
Bi5 O11 Ba2 . . 94.4(2) ?
Bi7 O11 Ba2 . . 94.0(2) ?
Ba3 O11 Ba2 2_666 . 97.70(14) ?
Bi5 O11 Ba1 . 2_666 84.91(18) ?
Bi7 O11 Ba1 . 2_666 85.08(17) ?
Ba3 O11 Ba1 2_666 2_666 90.31(18) ?
Ba2 O11 Ba1 . 2_666 172.0(2) ?
Bi5 O11 Ba4 . . 84.17(18) ?
Bi7 O11 Ba4 . . 84.20(17) ?
Ba3 O11 Ba4 2_666 . 173.5(2) ?
Ba2 O11 Ba4 . . 88.82(18) ?
Ba1 O11 Ba4 2_666 . 83.17(11) ?
Bi6 O12 Na8 . 1_565 166.6(2) ?
Bi6 O12 Ba4 . 2_566 95.3(2) ?
Na8 O12 Ba4 1_565 2_566 94.8(2) ?
Bi6 O12 Ba1 . . 94.0(2) ?
Na8 O12 Ba1 1_565 . 93.4(2) ?
Ba4 O12 Ba1 2_566 . 96.98(13) ?
Bi6 O12 Ba2 . 2_565 85.59(16) ?
Na8 O12 Ba2 1_565 2_565 85.57(17) ?
Ba4 O12 Ba2 2_566 2_565 90.61(17) ?
Ba1 O12 Ba2 . 2_565 172.4(2) ?
Bi6 O12 Ba3 . 1_554 84.54(17) ?
Na8 O12 Ba3 1_565 1_554 84.51(17) ?
Ba4 O12 Ba3 2_566 1_554 174.3(2) ?
Ba1 O12 Ba3 . 1_554 88.73(17) ?
Ba2 O12 Ba3 2_565 1_554 83.68(10) ?

